4.
iv
3.3 Physical Consequences of the Dirac Equation . . . . . . . . . . 61
3.3.1 Minimal length for the localisation of a relativistic par-
ticle . . . . . . . . . . . . . . . . . . . . . . . . . . . . 61
3.3.2 Velocity operator and “Zitterbewegung” . . . . . . . . 61
3.3.3 Klein tunneling and the absence of backscattering . . . 61
5.
Chapter 1
Introduction to Carbon
Materials
The experimental and theoretical study of graphene, two-dimensional (2D)
graphite, is an extremely rapidly growing ﬁeld of today’s condensed matter
research. A milestone was the experimental evidence of an unusual quan-
tum Hall eﬀect reported in September 2005 by two diﬀerent groups, the
Manchester group led by Andre Geim and a Columbia-Princeton collabora-
tion led by Philip Kim and Horst Stormer [1, 2]. Since this moment and
until March 2008, the beginning of the present series of lectures, almost 700
manuscripts with “graphene” in their title have been posted on the preprint
server www.arXiv.org (see Fig. 1.1).
The reasons for this enormous scientiﬁc interest are manyfold, but one
may highlight some major motivations. First, one may emphasise its possible
technological potential. One of the ﬁrst publications on graphene in 2004 by
the Geim group proved indeed the possibility of an electric ﬁeld eﬀect in
graphene, i.e. the possibility to control the carrier density in the graphene
sheet by simple application of a gate voltage [3]. This eﬀect is a fundamental
element for the design of electronic devices. Today’s silicon-based electronics
reaches its limits in miniaturisation, which is on the order of 50 nm for an
electric channel, whereas it has been shown that a narrow graphene strip
with a width of only a few nanometers may be used as a transistor [4],
i.e. the basic electronics component. One may therefore hope to improve
the miniaturisation by one order of magnitude when using graphene-based
electronics.
Apart from these promising technological applications, two major moti-
1
6.
2 Introduction to Carbon Materials
25
154
398
2006 2007
2006
before
100
200
300
400
Figure 1.1: Number of manuscripts with “graphene” in the title posted on the preprint
server. In interpreting these numbers, one must, however, consider that several publica-
tions on graphene appeared before 2006, e.g. in the framework of carbon-nanotube or
graphite research. At this moment, the name “graphene” was not commonly used.
vations for fundamental research may be emphasised. Graphene is the ﬁrst
truely 2D crystal ever observed in nature. This is remarkable because the
existence of 2D crystals has often been doubted in the past, namely due to
a theorem (Mermin-Wagner theorem) which states that a 2D crystal looses
its long-range order, and thus melts, at any small but non-zero temperature,
due to thermal ﬂuctuations. Furthermore, electrons in graphene show rel-
ativistic behaviour, and the system is therefore an ideal candidate for the
test of quantum-ﬁeld theoretical models which have been developed in high-
energy physics. Most promenently, electrons in graphene may be viewed as
massless charged fermions living in 2D space, particles one usually does not
encounter in our three-dimensional world. Indeed, all massless elementary
particles happen to be electrically neutral, such as photons or neutrinos.1
Graphene is therefore an exciting bridge between condensed-matter and high-
energy physics, and the research on its electronic properties unites scientists
with various thematic backgrounds. The discussion of graphene’s electronic
properties and how such relativistic eﬀects are revealed in electric transport
measurements is naturally a prominent part of the present lecture notes.
The interest in graphene is not only limited to the scientiﬁc community.
An important number of large-audience articles have recently been published.
The following list of (more or less serious) citations reveals this broad interest
1
The neutrino example is only partially correct. It has been shown that neutrinos must
indeed have a tiny non-zero mass.
7.
The Carbon Atom and its Hybridisations 3
“Electrons travel through it so fast that their behaviour is gov-
erned by the theory of relativity rather than classical physics.”
(The Economist, 2006)
“Inside every pencil, there is a neutron star waiting to get out.”
(New Scientist, 2006)
“We’ll have to rewrite the theory of metals for this problem.”
(Physics Today, 2006)
Notice that the last citation is from a leading scientist in the ﬁeld and may
indeed serve as a guideline for these lectures.2
1.1 The Carbon Atom and its Hybridisations
Carbon, the elementary constituent of graphene and graphite, is the 6th
element of the periodic table. Its atom is, therefore, built from 6 protons,
A neutrons, and 6 electrons, where A = 6 and 7 yield the stable isotopes
12
C and 13
C, respectively, and A = 8 characterises the radioactive isotope
14
C. The isotope 12
C, with a nuclear spin I = 0, is the most common one
in nature with 99% of all carbon atoms, whereas only 1% are 13
C with a
nuclear spin I = 1/2. There are only traces of 14
C (10−12
of all carbon
atoms) which β-decays into nitrogen 14
N. Although 14
C only occurs rarely,
it is an important isotope used for historical dating (radiocarbon). Due to
its half-life of 5 700 years, which corresponds to a reasonable time scale in
human history, measurement of the 14
C concentration of an organic material,
mainly wood, allows one to date its biological activity up to a maximum age
of roughly 80 000 years. In general, carbon is the elementary building block
of all organic molecules and, therefore, responsible for life on Earth.
In the atomic ground state, the 6 electrons are in the conﬁguration
1s2
2s2
2p2
, i.e. 2 electrons ﬁll the inner shell 1s, which is close to the nucleus
and which is irrelevant for chemical reactions, whereas 4 electrons occupy the
outer shell of 2s and 2p orbitals. Because the 2p orbitals (2px, 2py, and 2pz)
are roughly 4 eV higher than the 2s orbital, it is energetically favourable to
2
However, our aim is more modest – we do not intend to “rewrite” but rather to “apply”
the theory of metals to graphene.
8.
4 Introduction to Carbon Materials
2s
2p
1s
2p 2p
Energy
ground state
x y z
2s
2p
1s
2p 2px y z
excited state
( ~ 4 eV)
~ 4 eV
Figure 1.2: Electronic conﬁgurations for carbon in the ground state (left) and in the
excited state (right).
put 2 electrons in the 2s orbital and only 2 of them in the 2p orbitals (Fig
1.2). It turns out, however, that in the presence of other atoms, such as e.g.
H, O, or other C atoms, it is favourable to excite one electron from the 2s to
the third 2p orbital, in order to form covalent bonds with the other atoms.
The gain in energy from the covalent bond is indeed larger than the 4 eV
invested in the electronic excitation.
In the excited state, we therefore have four equivalent quantum-mechanical
states, |2s , |2px , |2py , and |2pz . A quantum-mechanical superposition of
the state |2s with n |2pj states is called spn
hybridisation, which play an
essential role in covalent carbon bonds.
1.1.1 sp1
hybridisation
In the sp1
hybridisation,3
the |2s state mixes with one of the 2p orbitals.
For illustration, we we have chosen the |2px state. A state with equal weight
from both original states, is obtained by the symmetric and anti-symmetric
combinations
|sp+ =
1
√
2
(|2s + |2px ) , |sp− =
1
√
2
(|2s − |2px ) .
The other states, |2py and |2pz , remain unaﬀected by this superposition.
The electronic density of the hybridised orbitals has the form of a club and
3
The superscript is often omitted, and one may alternatively use “sp hybridisation”.
9.
The Carbon Atom and its Hybridisations 5
000000000000000000000000000000000000000000000
000000000000000000000000000000000000000000000000000000000000000000000000000
000000000000000000000000000000000000000000000
111111111111111111111111111111111111111111111
111111111111111111111111111111111111111111111111111111111111111111111111111
111111111111111111111111111111111111111111111
000000000000000000000000000000000000000000000
000000000000000000000000000000000000000000000000000000000000000000000000000
000000000000000000000000000000000000000000000
111111111111111111111111111111111111111111111
111111111111111111111111111111111111111111111111111111111111111111111111111
111111111111111111111111111111111111111111111
000000000000000000000000000000000000000000000
000000000000000000000000000000000000000000000000000000000000000000000000000
000000000000000000000000000000000000000000000000000000000000
111111111111111111111111111111111111111111111
111111111111111111111111111111111111111111111111111111111111111111111111111
111111111111111111111111111111111111111111111111111111111111
000000000000000000000000000000000000000000000
000000000000000000000000000000000000000000000000000000000000000000000000000
000000000000000000000000000000000000000000000000000000000000
111111111111111111111111111111111111111111111
111111111111111111111111111111111111111111111111111111111111111111111111111
111111111111111111111111111111111111111111111111111111111111
|2s>
|2s> −|2p >
|2p >
|sp >x
x |sp >
−
+
(a)
CC
H H
(b)
bondσ
Figure 1.3: (a) Schematic view of the sp1
hybridisation. The ﬁgure shows on the r.h.s.
the electronic density of the |2s and |2px orbitals and on the l.h.s. that of the hybridised
ones. (b) Acetylene molecule (H–C≡C–H). The propeller-like 2py and 2pz orbitals of the
two C atoms strengthen the covalent σ bond by forming two π bonds (not shown).
10.
6 Introduction to Carbon Materials
C
C
C
C
C
C
H
H
H
H
H
H
000000000000000000000000
000000000000000000000000
000000000000000000000000000000000000
000000000000000000000000
000000000000000000000000000000000000
000000000000000000000000
000000000000000000000000000000000000
000000000000
111111111111111111111111
111111111111111111111111
111111111111111111111111111111111111
111111111111111111111111
111111111111111111111111111111111111
111111111111111111111111
111111111111111111111111111111111111
111111111111
0000000000000000000000
0000000000000000000000
000000000000000000000000000000000
0000000000000000000000
000000000000000000000000000000000
0000000000000000000000
000000000000000000000000000000000
1111111111111111111111
1111111111111111111111
111111111111111111111111111111111
1111111111111111111111
111111111111111111111111111111111
1111111111111111111111
111111111111111111111111111111111
000000000000
000000000000
000000000000000000
000000000000
000000000000000000
000000000000
000000000000000000
000000000000
000000000000000000
000000000000
000000000000
111111111111
111111111111
111111111111111111
111111111111
111111111111111111
111111111111
111111111111111111
111111111111
111111111111111111
111111111111
111111111111
120 0
(a)
(c)
(b)
(d)
Figure 1.4: (a) Schematic view of the sp2
hybridisation. The orbitals form angles of
120o
. (b) Benzene molecule (C6H6). The 6 carbon atoms are situated at the corners of
a hexagon and form covalent bonds with the H atoms. In addition to the 6 covalent σ
bonds between the C atoms, there are three π bonds indicated by the doubled line. (c)
The quantum-mechanical ground state of the benzene ring is a superposition of the two
conﬁgurations which diﬀer by the position of the π bonds. The π electrons are, thus,
delocalised over the ring. (d) Graphene may be viewed as a tiling of benzene hexagons,
where the H atoms are replaced by C atoms of neighbouring hexagons and where the π
electrons are delocalised over the whole structure.
is elongated in the +x (−x) direction for the |sp+ (|sp− ) states [Fig. 1.3
(a)]. This hybridisation plays a role, e.g., in the formation of the acetylene
molecule H–C≡C–H, where overlapping sp1
orbitals of the two carbon atoms
form a strong covalent σ bond [Fig. 1.3 (b)]. The remaining unhybridised 2p
orbitals are furthermore involved in the formation of two additional π bonds,
which are weaker than the σ bond.
1.1.2 sp2
hybridisation – graphitic allotopes
In the case of a superposition of the 2s and two 2p orbitals, which we may
choose to be the |2px and the |2py states, one obtains the planar sp2
hy-
11.
The Carbon Atom and its Hybridisations 7
bridisation. The three quantum-mechanical states are given by
|sp2
1 =
1
√
3
|2s −
2
3
|2py ,
|sp2
2 =
1
√
3
|2s +
2
3
√
3
2
|2px +
1
2
|2py , (1.1)
|sp2
3 = −
1
√
3
|2s +
2
3
−
√
3
2
|2px +
1
2
|2py .
These orbitals are oriented in the xy-plane and have mutual 120o
angles
[Fig. 1.4 (a)]. The remaining unhybridised 2pz orbital is perpendicular to
the plane.
A prominent chemical example for such hybridisation is the benzene
molecule the chemical structure of which has been analysed by August Kekul´e
in 1865 [5]. The molecule consists of a hexagon with carbon atoms at the
corners linked by σ bonds [Fig. 1.4 (b)]. Each carbon atom has, furthermore,
a covalent bond with one of the hydrogen atoms which stick out from the
hexagon in a star-like manner. In addition to the 6 σ bonds, the remaining
2pz orbitals form 3 π bonds, and the resulting double bonds alternate with
single σ bonds around the hexagon. Because a double bond is stronger than
a single σ bond, one may expect that the hexagon is not perfect. A double
bond (C=C) yields indeed a carbon-carbon distance of 0.135 nm, whereas it
is 0.147 nm for a single σ bond (C–C). However, the measured carbon-carbon
distance in benzene is 0.142 nm for all bonds, which is roughly the average
length of a single and a double bond. This equivalence of all bonds in ben-
zene was explained by Linus Pauling in 1931 within a quantum-mechanical
treatment of the benzene ring [6]. The ground state is indeed a quantum-
mechanical superposition of the two possible conﬁgurations for the double
bonds, as shown schematically in Fig. 1.4 (c).
These chemical considerations indicate the way towards carbon-based
condensed matter physics – any graphitic compound has indeed a sheet of
graphene as its basic constituent. Such a graphene sheet may be viewed sim-
ply as a tiling of benzene hexagons, where one has replaced the hydrogen by
carbon atoms to form a neighbouring carbon hexagon [Fig. 1.4 (d)]. How-
ever, graphene has remained the basic constituent of graphitic systems during
a long time only on the theoretical level. From an experimental point of view,
graphene is the youngest allotope and accessible to physical measurements
12.
8 Introduction to Carbon Materials
(a) (b)
(c)
(e)
(d)
Figure 1.5: Graphitic allotopes (a) Piece of natural graphite. (b) Layered structure of
graphite (stacking of graphene layers). (c) 0D allotope: C60 molecule. (d) 1D allotope:
single-wall carbon nanotube. (e) Optical image of a carbon nanotube.
only since 2004.
Historically, the longest known allotope is 3D graphite [Fig. 1.5 (a)].
Graphite was discovered in a mine near Borrowdale in Cumbria, England in
the 16th century, and its use for marking and graphical purposes was almost
immediately noticed. Indeed, the nearby farmers used graphite blocks from
the mine for marking their sheep. Due to its softness and dark color, graphite
was considered during a long time as some particular type of lead. The full
name “lead pencil” still witnesses this historical error.4
That graphite was
formed from carbon atoms was discovered by the Swedish-German pharma-
cist Carl Wilhelm Scheele in the middle of the 18th century. But it was the
German chemist Abraham Gottlob Werner in 1789 who coined the material
by its current name “graphite”, thus emphasising its main use for graphical
purposes.5
Graphite may be viewed as a stacking of graphene sheets [Fig. 1.5 (b)]
that stick together due to the van der Waals interaction, which is much
4
The graphitic core of a pencil is still called “lead”, and the German name for “pencil”
is “Bleistift”, “Blei” being the German name for lead.
5
The term is derived from the Greek word γραϕǫιν (“graphein”, to draw, to write).
13.
The Carbon Atom and its Hybridisations 9
weaker than the inplane covalent bonds. This physical property explains the
graphic utility of the material: when one writes with a piece of graphite,
i.e. when it is scratched over a suﬃciently rough surface, such as a piece of
paper, thin stacks of graphene sheets are exfoliated from bulk graphite and
now stick to the surface. This is possible due to the above-mentioned weak
van der Waals interaction between the graphene sheets.
The 0D graphitic allotope (fullerenes) has been discovered in 1985 by
Robert Curl, Harold Kroto, and Richard Smalley [7]. Its most prominent
representative is the C60 molecule which has the form of a football and is also
called “buckyball”. It consists of a graphene sheet, where some hexagons are
replaced by pentagons, which cause a crumbling of the sheet and the ﬁnal
formation of a graphene sphere [Fig. 1.5 (c)]. Its existance had been predicted
before, in 1970, by the Japanese theoretician Eiji Ozawa [8].
Carbon nanotubes, the 1D allotope, may be viewed as graphene sheets
which are rolled up [Fig. 1.5 (d) and (e)], with a diameter of several nano-
meters. One distinguishes single-wall from multi-wall nanotubes, according
to the number of rolled up graphene sheets. The discovery of carbon nan-
otubes is most often attributed to Sumio Iijima and his 1991 publication in
Nature [9]. Recently, doubts about this attribution have been evoked because
it seems that carbon nanotubes had a longer history in the community of ma-
terial scientists [10]. Indeed, a publication by the Soviet scientists Radushke-
vich and Lukyanovich in 1952 contained a transmission electron microscope
image showing carbon nanotubes [11]. It is, however, the merit of the 1991
Iijima paper to have attracted the interest of the condensed matter physics
community to carbon nanotubes and to have initiated an intense research on
this compound, also in the prospect of nanotechnological applications.
1.1.3 sp3
hybridisation – diamonds
If one superposes the 2s and all three 2p orbitals, one otains the sp3
hybridi-
sation, which consists of four club-like orbitals that mark a tetrahedron. The
orbitals form angles of 109.5o
degrees [Fig. 1.6 (a)]. A chemical example
for this hybridisation is methane (CH4), where the four hybridised orbitals
are used to form covalent bonds with the 1s hydrogen atoms. In condensed
matter physics, the 2p3
hybridisation is at the origin of the formation of di-
amonds, when liquid carbon condenses under high pressure. The diamond
lattice consists of two interpenetrating face-center-cubic (fcc) lattices, with
a lattice spacing of 0.357 nm, as shown in Fig. 1.6 (b).
14.
10 Introduction to Carbon Materials
000
000
000
000
000
000
000
000
000
000
000
000
000
000
111
111
111
111
111
111
111
111
111
111
111
111
111
111
00000
00000
00000
00000
00000
11111
11111
11111
11111
11111
0000000
0000000
0000000
0000000
0000000
0000000
0000000
0000000
1111111
1111111
1111111
1111111
1111111
1111111
1111111
1111111
000000
000000
000000
000000
000000
000000
000000
000000
000000
000000
000000
000000
111111
111111
111111
111111
111111
111111
111111
111111
111111
111111
111111
111111
109.5o
(a) (b)
0.357nm
Figure 1.6: (a) sp3
hybridisation with 109.5o
angle between the four orbitals. (b) Crystal
structure of diamond (two interpenetrating fcc lattices).
Although they consist of the same atomic ingredient, namely carbon,
the 3D graphite and diamond crystals are physically extremely diﬀerent.
Graphite, as described above, is a very soft material due to its layered struc-
ture, whereas diamond is one of the hardest natural materials because all
bonds are covalent σ bonds. The fact that all 4 valence electrons in the outer
atomic shell are used in the formation of the σ bondes is also the reason for
diamond being an insulator with a large band gap of 5.47 eV. In contrast
to insulating diamond, the electrons in the weaker π bonds in graphite are
delocalised and, thus, yield good electronic conduction properties.
1.2 Crystal Structure of Graphene and Graphite
1.2.1 Graphene’s honeycomb lattice
As already mentioned in the last section, the carbon atoms in graphene con-
dense in a honeycomb lattice due to their sp2
hybridisation. The honeycomb
lattice is not a Bravais lattice because two neighbouring sites are not equiva-
lent. Fig. 1.7 (a) illustrates indeed that a site on the A sublattice has nearest
neighbours (nn) in the directions north-east, north-west, and south, whereas
a site on the B sublattice has nns in the directions north, south-west, and
south-east. Both A and B sublattices, however, are triangular6
Bravais lat-
tices, and one may view the honeycomb lattice as a triangular Bravais lattice
with a two-atom basis (A and B). The distance between nn carbon atoms
is 0.142 nm, which is the average of the single (C–C) and double (C=C)
6
The triangular lattice is sometimes also called hexagonal lattice.
15.
Crystal Structure of Graphene and Graphite 11
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
00000000000000000
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
11111111111111111
: A sublattice : B sublattice
a
a
a
a
δ
δ
δ
(a) (b)
KK’
K K’
K’K M’’
M’
M
M’’
M’
M *
*
Γ
a=0.142 nm
y
x
2
1
1
2
2
1
3
Figure 1.7: (a) Honeycomb lattice. The vectors δ1, δ2, and δ3 connect nn carbon atoms,
separated by a distance a = 0.142 nm. The vectors a1 and a2 are basis vectors of the tri-
angular Bravais lattice. (b) Reciprocal lattice of the triangular lattice. Its primitive lattice
vectors are a∗
1 and a∗
2. The shaded region represents the ﬁrst Brillouin zone (BZ), with
its centre Γ and the two inequivalent corners K (black squares) and K′
(white squares).
The thick part of the border of the ﬁrst BZ represents those points which are counted in
the deﬁnition such that no points are doubly counted. The ﬁrst BZ, deﬁned in a strict
manner, is, thus, the shaded region plus the thick part of the border. For completeness,
we have also shown the three inequivalent cristallographic points M, M′
, and M′′
(white
triangles).
covalent σ bonds, as in the case of benzene.
The three vectors which connect a site on the A sublattice with a nn on
the B sublattice are given by
δ1 =
a
2
√
3ex + ey , δ2 =
a
2
−
√
3ex + ey , δ3 = −aey, (1.2)
and the triangular Bravais lattice is spanned by the basis vectors
a1 =
√
3aex and a2 =
√
3a
2
ex +
√
3ey . (1.3)
The modulus of the basis vectors yields the lattice spacing, ˜a =
√
3a = 0.24
nm, and the area of the unit cell is Auc =
√
3˜a2
/2 = 0.051 nm2
. The density
of carbon atoms is, therefore, nC = 2/Auc = 39 nm−2
= 3.9 × 1015
cm−2
.
Because there is one π electron per carbon atom that is not involved in a
covalent σ bond, there are as many valence electrons than carbon atoms, and
their density is, thus, nπ = nC = 3.9 × 1015
cm−2
. As is discussed in the
following chapter, this density is not equal to the carrier density in graphene,
which one measures in electrical transport measurements.
16.
12 Introduction to Carbon Materials
The reciprocal lattice, which is deﬁned with respect to the triangular
Bravais lattice, is depicted in Fig. 1.7 (b). It spanned by the vectors
a∗
1 =
2π
√
3a
ex −
ey
√
3
and a∗
2 =
4π
3a
ey. (1.4)
Physically, all sites of the reciprocal lattice represent equivalent wave vectors.
Any wave – be it a vibrational lattice excitation or a quantum-mechanical
electronic wave packet – propagating on the lattice with a wave vector diﬀer-
ing by a reciprocal lattice vector has indeed the same phase up to a multiple
of 2π, due to the relation
ai · a∗
j = 2πδij (1.5)
(for i, j = 1, 2) between direct and reciprocal lattice vectors. The ﬁrst Bril-
louin zone [BZ, shaded region and thick part of the border of the hexagon in
Fig. 1.7 (b)] represents a set of inequivalent points in the reciprocal space,
i.e. of points which may not be connected to one another by a reciprocal
lattice vector, or else of physically distinguishable lattice excitations. The
long wavelength excitations are situated in the vicinity of the Γ point, in
centre of the ﬁrst BZ. Furthermore, one distinguishes the six corners of the
ﬁrst BZ, which consist of the inequivalent points K and K′
represented by
the vectors
±K = ±
4π
3
√
3a
ex. (1.6)
The four remaining corners [shown in gray in Fig. 1.7 (b)] may indeed be con-
nected to one of these points via a translation by a reciprocal lattice vector.
These cristallographic points play an essential role in the electronic proper-
ties of graphene because their low-energy excitations are centered around the
two points K and K′
, as is discussed in detail in the following chapter. We
emphasise, because of some confusion in the litterature on this point, that
the inequivalence of the two BZ corners, K and K′
, has nothing to do with
the presence of two sublattices, A and B, in the honeycomb lattice. The
form of the BZ is an intrinsic property of the Bravais lattice, independent
of the possible presence of more than one atom in the unit cell. For com-
pleteness, we have also shown, in Fig. 1.7 (b), the three crystallographically
inequivalent M points in the middle of the BZ edges.
17.
Crystal Structure of Graphene and Graphite 13
δ1
1−δ
(b)(a)
x
y
z
Figure 1.8: Two possibilities for stacking two graphene layers. The symbols correspond
to the following lattice sites: black circles are A sites in the lower layer, black triangles
B sites in the lower layer, white circles A’ sites in the upper layer, and white triangles B’
sites in the upper layer. (a) The upper layer is translated by δ1 with respect to the lower
one; the A’ sites are on top of the B sites. (b) The upper layer is translated by −δ1 with
respect to the lower one; the B’ sites are on top of the A sites.
1.2.2 Graphene stacking – the diﬀerent forms of graphite
Graphite consists of stacked graphene layers. One distinguishes crystal (or-
dered) graphite, with two diﬀerent basic stacking orders, from turbostratic
graphite with a certain amount of disorder in the stacking.
To illustrate the ordering of graphene layers in crystal graphite, we ﬁrst
consider only two graphene layers (bilayer graphene). The distance between
layers is roughly d = 2.4a = 0.34 nm, and the stacking is such that there are
atoms in the upper layer placed at the hexagon centres of the lower layer.
The layers are, thus, translated with respect to each other, and one may
distinguish two diﬀerent patterns, as shown in Fig. 1.8. The displacement
is given by either δi or −δi, where one may choose any of the nn vectors
(1.2) with i = 1, 2, or 3. For the choice δi, one obtains a conﬁguration where
the A’ atoms of the upper layer are on top of the B atoms of the lower one
[Fig. 1.8 (a)], and for a translation of −δi, the B’ atoms in the upper layer
are on top of A atoms in the lower one [Fig. 1.8 (b)]. Notice that the two
conﬁgurations, both of which contain now four atoms (A, B, A’, and B’) per
unit cell, are equivalent if one has a reﬂexion symmetry in the perpendicular
axis, z → −z.
Although physically not relevant in the bilayer case, this diﬀerence in the
stackingturns out to be important when considering crystal graphite with an
18.
14 Introduction to Carbon Materials
inﬁnity of stacked layers. Let us consider the situation where the second layer
is translated with respect to the ﬁrst by δi. The third layer may be chosen
to be translated with respect to the second either by −δi, in which case its
sites coincide with those of the ﬁrst one, or again by δi, where the atomic
conﬁguration of the ﬁrst layer is not recovered. In the ﬁrst case, one therefore
obtains an ABA stacking, whereas the stacking is ABC in the second case.
In general, one distingushes two types of ordering:
1. All layers are translated with respect to their lower neighbour by δi.
One obtains a rhombohedral stacking, which is also called ABC stack-
ing because one needs three layers to recover the atomic conﬁguration
of the original layer. There are, thus, 6 atoms per unit cell which has
an extension of 3d in the z-direction (β-graphite).
2. If the sign of the translation alternates, i.e. δi, −δi, δi, −δi, ..., when
stacking the graphene layers, one obtains a hexagonal (or else AB or
Bernal) stacking. Here, one has 4 atoms per unit cell which has a height
of 2d in the z-direction (α-graphite).
In principle, it is possible to have some randomness in the stacking, i.e.
ABC parts may randomly substitute AB parts when considering α-graphite.
However, a crystalline AB stacking occurs most often in nature, with about
30% of ABC-stacked graphite.
In the case of turbostratic graphite, one may distinguish translational dis-
order from rotational disorder in the stacking. Generally, the graphene layers
are much less bound together in turbostratic than in crystalline graphite, such
that turbostratic graphite is a better lubriﬁcant.
As an example of rotational disorder, we consider two graphene layers
which are rotated by an angle
φ =
a1 · a′
1
|a1||a′
1|
= ex · e′
x
with respect to each other, where a′
1 denotes the lattice vector in the upper
graphene layer corresponding to a1 in the lower one. If the angle fulﬁls certain
comensurability conditions, one obtains a so-called Moir´e pattern, with a
larger unit cell as depictecd in Fig. 1.9. The Moir´e pattern reproduces a
(larger) honeycomb lattice.
19.
Crystal Structure of Graphene and Graphite 15
φ
Figure 1.9: Moir´e pattern obtained by stacking two honeycomb lattices (gray) with a
relative (chiral) angle φ. One obtains a hexagonal superstructure indicated by the black
hexagons.
20.
16 Introduction to Carbon Materials
(a) (b)
Figure 1.10: (a) AFM image of a graphene ﬂake on a SiO2 substrate. (b) Transmission-
electron-microscopic image of free-hanging graphene. Both pictures have been taken by
the Manchester group.
1.3 Fabrication of Graphene
We brieﬂy review the two techniques used in fabricating graphene, mechan-
ical exfoliation of graphene from bulk graphite and graphitisation of epitax-
ially grown SiC crystals. The resulting graphene probes have similar, but
not always equal, physical properties. It is therefore important to describe
both systems separately and to clearly indicate on what type of graphene,
exfoliated or epitaxial, a particular measurement is performed. A systematic
comparison of both graphene types is still an open research ﬁeld.
1.3.1 Exfoliated graphene
The mechanical exfoliation technique, elaborated mainly by the Manchester
group, consistsy of peeling a layered material [13]. In the case of graphite, it
uses its primary graphical capacity, which we have already alluded to above:
if one scratches a piece of graphite on a substrate, thin graphite stacks are
exfoliated from the bulk and left behind on the substrate. Most of these thin
stacks comprise several (tens or hundreds) of graphene sheets, but a few of
them only consist of a single graphene layer. The fabrication of graphene is,
thus, extremely simple, and we produce single layers of graphene whenever
we write with a pencil of suﬃciently high graphitic quality.7
In practice, one does not use a pencil to fabricate graphene layers, but one
prepares very thin samples by peeling a small graphite crystallite in a piece
7
Not all pencils are of the required quality. The graphite lead of most pencils contains
normally a certain amount of clay impurities.
21.
Fabrication of Graphene 17
of folded scotchtape. Each time one peels away the tape, the graphite ﬂake
is cleaved into two parts and thus becomes thinner. After several cycles,
the scotchtape with the graphene sheets stuck to it is glued to the SiO2
substrate, prepared by a mix of hydrochloric acid and hydrogen peroxide
to accept better the graphene sheets from the scothtape. When the tape is
carefully peeled away, the graphene sheets remain glued to the substrate.
The main problem consists of the identiﬁcation of the few single graphene
layers, which are randomly distributed on the substrate. A deﬁnitve identi-
ﬁcation may be achieved by atomic-force microscopy (AFM), the scanning
capacity of which is unfortunately limited to a very small surface during a
reasonable time. One therefore needs to have a hint of where to search for
mono-layer graphene. This hint comes from a ﬁrst (optical) glance at the
substrate. The 300 nm thick SiO2 substrate, which was originally used by
the Manchester group and which is now most common, turns out to yield an
optimal contrast such that one may, by optical meanse, identify mono-layer
graphene sheets with a high probability. AFM imaging is then used to con-
ﬁrm this ﬁrst glance. An example of such AFM image is shown in Fig. 1.10
(a). Notice that it has been shown that one may also depose an exfoliated
graphene sheet on a scaﬀold such that it is free-hanging over a rather large
surface of several µm2
[Fig. 1.10 (b)].
The exfoliation technique is not limited to graphite, but may also be
used in the fabrication of ultra-thin samples from other layered crystals.
The Manchester group has indeed shown that one may, by this technique,
fabricate e.g. single layer BN, NbSe2, Bi2Sr2CaCu2Ox, and MoS2 crystallites
of a typical size of several µm2
[13]. The exfoliation technique is, therefore,
extremely promising in the study of truly 2D crystals.
One may, furthermore, control the carrier density in the metallic 2D crys-
tals, such as graphene, by the electric ﬁeld eﬀect; the 300 nm thick insulating
SiO2 layer is indeed on top of a positively doped metallic Si substrate, which
serves as a backgate. The combined system graphene-SiO2-backgate may,
thus, be viewed as a capacitor (see Fig. 1.11) the capacity of which is
C =
Q
Vg
=
ǫ0ǫA
d
, (1.7)
where Q = en2DA is the capacitor charge, in terms of the total surface A,
Vg is the gate voltage, d = 300 nm is the thickness of the SiO2 layer with
the dielectric constant ǫ = 3.7. The ﬁeld-eﬀect induced 2D carrier density is
22.
18 Introduction to Carbon Materials
0000000000000000000000000000000
0000000000000000000000000000000
0000000000000000000000000000000
0000000000000000000000000000000
0000000000000000000000000000000
0000000000000000000000000000000
0000000000000000000000000000000
0000000000000000000000000000000
0000000000000000000000000000000
0000000000000000000000000000000
0000000000000000000000000000000
0000000000000000000000000000000
0000000000000000000000000000000
0000000000000000000000000000000
0000000000000000000000000000000
0000000000000000000000000000000
0000000000000000000000000000000
1111111111111111111111111111111
1111111111111111111111111111111
1111111111111111111111111111111
1111111111111111111111111111111
1111111111111111111111111111111
1111111111111111111111111111111
1111111111111111111111111111111
1111111111111111111111111111111
1111111111111111111111111111111
1111111111111111111111111111111
1111111111111111111111111111111
1111111111111111111111111111111
1111111111111111111111111111111
1111111111111111111111111111111
1111111111111111111111111111111
1111111111111111111111111111111
1111111111111111111111111111111
2300 nm
SiO
graphene (2D metal)
(insulator)
doped Si (metal)
Vg
Figure 1.11: Schematic view of graphene on a SiO2 substrate with a doped Si (metallic)
backgate. The system graphene-SiO2-backgate may be viewed as a capacitor the charge
density of which is controled by a gate voltage Vg.
thus given by
n2D = αVg with α ≡
ǫ0ǫ
ed
≃ 7.2 × 1010 cm−2
V
. (1.8)
The gate voltage may vary roughly between −100 and 100 V, such that one
may induce maximal carrier densities on the order of 1012
cm−2
, on top of
the intrinsic carrier density which turns out to be zero in graphene, as will be
discussed in the next chapter. At gate voltages above ±100 V, the capacitor
breaks down (electrical breakdown).
1.3.2 Epitaxial graphene
An alternative method to fabricate graphene has been developed by the At-
lanta group, led by Walt de Heer and Claire Berger [14]. It consists of expos-
ing an epitaxially grown hexagonal (4H or 6H-) SiC crystal8
to temperatures
of about 1300o
C in order to evaporate the less tightly bound Si atoms from
the surface. The remaining carbon atoms on the surface form a graphitic
layer (graphitsation). The physical properties of this graphitic layer depend
on the chosen SiC surface. In the case of the Si-terminated (0001) surface,
the graphitisation process is slow, and one may thus control the number of
formed graphene layers (usually one or two). The resulting electron mobility,
8
SiC exists also in several other crystal structures, such as the zinc blende structure
(3C-SiC), i.e. a diamond structure with diﬀerent atom types on the two distinct fcc
sublattices.
23.
Fabrication of Graphene 19
0000000000000000000000000000000000000
0000000000000000000000000000000000000
00000000000000000000000000000000000000000000000000000000000000000000000000
0000000000000000000000000000000000000
0000000000000000000000000000000000000
0000000000000000000000000000000000000
00000000000000000000000000000000000000000000000000000000000000000000000000
0000000000000000000000000000000000000
0000000000000000000000000000000000000
0000000000000000000000000000000000000
00000000000000000000000000000000000000000000000000000000000000000000000000
0000000000000000000000000000000000000
0000000000000000000000000000000000000
0000000000000000000000000000000000000
00000000000000000000000000000000000000000000000000000000000000000000000000
0000000000000000000000000000000000000
0000000000000000000000000000000000000
0000000000000000000000000000000000000
1111111111111111111111111111111111111
1111111111111111111111111111111111111
11111111111111111111111111111111111111111111111111111111111111111111111111
1111111111111111111111111111111111111
1111111111111111111111111111111111111
1111111111111111111111111111111111111
11111111111111111111111111111111111111111111111111111111111111111111111111
1111111111111111111111111111111111111
1111111111111111111111111111111111111
1111111111111111111111111111111111111
11111111111111111111111111111111111111111111111111111111111111111111111111
1111111111111111111111111111111111111
1111111111111111111111111111111111111
1111111111111111111111111111111111111
11111111111111111111111111111111111111111111111111111111111111111111111111
1111111111111111111111111111111111111
1111111111111111111111111111111111111
1111111111111111111111111111111111111
00000000000000000000000000000000000001111111111111111111111111111111111111
00000000000000000000000000000000000001111111111111111111111111111111111111
00000000000000000000000000000000000001111111111111111111111111111111111111
SiC substrate
buffer
layer
layers
graphene0.39 nm
0.39 nm
0.38 (0.39) nm
0.20 (0.17) nm
(a) (b)
Figure 1.12: Epitaxial Graphene. (a) Schematic view on epitaxial graphene. On top
of the SiC substrate, a graphitic layer. It consists of several one-atom thick caron layers.
The ﬁrst one is a buﬀer layer, which is tightly bound to the substrate, at a distance of 0.2
(0.17) nm for a Si- (C-)terminated surface. The graphene layers are formed on top of this
buﬀer layer at a distance of 0.38 (0.39) nm, and they are equally spaced by 0.39 nm. (b)
AFM image of epitaxial graphene on C-terminated SiC substrate. The steps those of the
SiC substrate. The 5-10 graphene layers lie on the substrate similar to a carpet which has
folds visible as white lines on the image.
however, turns out to be rather low, such that the Si-terminated surface is
less chosen for the fabrication of samples used in transport measurements.
For a C-terminated (000¯1) surface, the graphitisation process is very fast,
and a large number of graphene layers are formed (up to 100). In contrast
to epitaxial graphene on the Si-terminated surface, the electron mobility is,
here, rather high.
In contrast to exfoliated graphene, the SiC substrate must be consid-
ered as an integral part of the whole system of epitaxial graphene. It is
indeed the mother compound, and the ﬁrst graphitic layer formed during the
graphitisation process is tightly bound to the SiC substrate (Fig. 1.12). The
distance between this layer and the substrate has been estimated numerically
to be 0.20 nm for a Si-terminated surface and 0.17 nm for a C-terminated
surface [15]. These distances are much smaller than the distance between
graphene sheets in crystalline graphite (2.4a = 0.34 nm). 0.38 (0.39) nm
above this buﬀer layer for Si- (C-)terminated SiC, several graphene layers
are formed, which are separated by a distance of 0.39 nm. These character-
istic distances are roughly 20% larger than the layer distances in crystalline
graphite, and one may therefore expect them to be less tightly bound. The
above-mentioned numerical values for the distances have been conﬁrmed by
X-ray measurements [15].
24.
20 Introduction to Carbon Materials
Furthermore, X-ray diﬀraction measurements have revealed a certain
amount of rotational disorder in the stacking of the graphene layers [16].
This, together with the rather large spacing between the graphene sheets on
top of the buﬀer layer, corroborates the view that the graphitic layer on the
SiC substrate consists indeed of almost independent graphene layers rather
than of a thin graphite ﬂake. However, the charge is not homogeneously
distributed between the diﬀerent graphene layers – it turns out that the
graphene layer,9
which is closest to the substrate, is electron-doped due to a
charge transfer from the bulk SiC, whereas the subsequent layers are hardly
charged. As will be discussed in the following chapters, this inhomogeneous
charge distribution in epitaxial graphene may be at the origin of diﬀerent
results in transport measurements when compared with exfoliated graphene
and theoretical predictions.
9
We refer to the layers on top of the buﬀer layer when using the term “graphene”. The
buﬀer layer may not be counted due to its tight bonding to the SiC substrate.
25.
Chapter 2
Electronic Band Structure of
Graphene
As we have discussed in the introduction, three electrons per carbon atom in
graphene are involved in the formation of strong covalent σ bonds, and one
electron per atom yields the π bonds. The π electrons happen to be those re-
sponsible for the electronic properties at low energies, whereas the σ electrons
form energy bands far away from the Fermi energy. This chapter is, thus,
devoted to a discussion of the energy bands of π electrons within the tight-
binding approximation, which was originally calculated for the honeycomb
lattice by P. R. Wallace in 1947 [17]. We do not consider the σ electrons,
here, and refer the interested reader to the book by Saito, Dresselhaus, and
Dresselhaus for a tight-binding calculation of the energy bands formed by
the σ electrons [12], which are far away from the Fermi level.
The chapter consists of two sections. The ﬁrst one is devoted to the cal-
culation of the π energy bands in graphene, where one is confronted with
the problem of two atoms per unit cell. After a brief discussion of Bloch’s
theorem, and a formal solution of the tight-binding model, we calculate the
energy dispersion of π electrons in graphene, taking into account nearest-
neighbour (nn) and next-nearest-neighbour (nnn) hopping and nn overlap
corrections. The second section consists of the continuum limit, which de-
scribes the low-energy properties of electrons in graphene.
21
26.
22 Electronic Band Structure of Graphene
2.1 Tight-Binding Model for Electrons on the
Honeycomb Lattice
The general idea of the tight-binding model is to write down a trial wave-
function constructed from the orbital wavefunctions, φ(a)
(r − Rj), of the
atoms forming a particular lattice described by the (Bravais) lattice vectors
Rj = mja1 +nja2, where mj and nj are integers.1
In addition, the trial wave-
function must reﬂect the symmetry of the underlying lattice, i.e. it must be
invariant under a translation by any arbitrary lattice vector Ri. We con-
sider, for simplicity in a ﬁrst step, the case of a Bravais lattice with one atom
per unit cell and one electron per atom. The Hamiltonian for an arbitrary
electron, labelled by the integer l, is given by
Hl = −
¯h2
2m
∆l +
N
j=1
V (rl − Rj), (2.1)
where ∆l = ∇2
l is the 2D Laplacian operator, in terms of the 2D gradient
∇l = ∂/∂xl + ∂/∂yl with respect to the electron’s position rl = (xl, yl), and
m is the electron mass. Each ion on site Rj yields an electrostatic potential
felt by the electron, and its overall potential energy N
j V (rl −Rj), where N
is the number of lattice sites, is, therefore, a periodic function with respect
to an arbitrary translation by a lattice vector Ri in the thermodynamic limit
N → ∞. The total Hamiltonian is the sum over all electrons,
H =
N
l
Hl, (2.2)
if we suppose one electron per lattice site, as mentioned above.
The tight-binding approach is based on the assumption that the electron l
is originally bound to a particular ion at the lattice site Rl, i.e. it is described
to great accuracy by a bound state of the (atomic) Hamiltonian
Ha
l = −
¯h2
2m
∆l + V (rl − Rl),
whereas the contributions to the potential energy ∆V = N
j=l V (rl−Rj) from
the other ions at the sites Rj, j = l, may be treated perturbatively. The
1
Because we are interested in 2D lattices, we limit the discussion to two dimensions,
the generalisation to arbitrary dimensions being straight-forward.
27.
Tight-Binding Model for Electrons on the Honeycomb Lattice 23
bound state of Ha
l is described by the above-mentioned atomic wavefunction
φ(a)
(r − Rj).
2.1.1 Bloch’s theorem
Another ingredient, apart from the atomic wavefunction, of the trial wave-
function is a symmetry consideration – the trial wavefunction must respect
the discrete translation symmetry of the lattice. This is the essence of Bloch’s
theorem. In quantum mechanics, a translation by a lattice vector Ri may be
described by the operator
TRi
= e
i
¯h
ˆp·Ri
, (2.3)
in terms of the momentum operator ˆp, which needs to be appropriately
deﬁned for the crystal and which we may call quasi-momentum operator,
as will become explicit below. The symmetry operator, because it describes
a symmetry operation under which the physical problem is left invariant,
commutes with the full Hamiltonian (2.2), [TRi
, H] = 0. The eigenstates of
H are, therefore, necessarily also eigenstates of TRi
, for any lattice vector Ri,
and the momentum p, which is the eigenvalue of the momentum operator
ˆp, is a good quantum number. Because of the relation (1.5) between the
basis vectors of the direct and the reciprocal lattices, this momentum is
only deﬁned modulo a reciprocal lattice vector Gj = m∗
j a∗
1 + n∗
j a∗
2, where
m∗
j and n∗
j are arbitrary integers. Indeed, if we had chosen the momentum
operator ˆp′
= ˆp + ¯hGj instead of ˆp in the deﬁnition (2.3) of the discrete
translation operator, we would have simply multiplied it with a factor of
exp(iGj ·Ri) = exp(i2πn) = 1 because of the integer value n = m∗
j mi +n∗
j ni.
We, thus, need to identify, as pointed out in the last chapter, identify all
momenta which diﬀer by a reciprocal lattice vector, and it is more convenient
to speak of a quasi-momentum p = ¯hk, which is restricted to the ﬁrst BZ.
The trial wavefunction, constructed from the atomic orbital wavefunc-
tions φ(a)
(r − Rj),
ψk(r) =
Rj
eik·Rj
φ(a)
(r − Rj) (2.4)
fulﬁls the above-mentioned requirements, i.e. it is an eigenstate of the trans-
lation operator (2.3).2
That the wavefunction (2.4) is indeed an eigenstate
2
The sum Rj
is a short notation for mj ,nj
and runs over all 2D lattice vectors
Rj = mja1 + nja2, in the thermodynamic limit of an inﬁnite lattice.
28.
24 Electronic Band Structure of Graphene
of TRi
may be seen from
TRi
ψk(r) = ψk(r + Ri)
=
Rj
eik·Rj
φ(a)
[r − (Rj − Ri)]
= eik·Ri
Rm
eik·Rm
φ(a)
(r − Rm) = eik·Ri
ψk(r),
where the ﬁrst line reﬂects the translation by the lattice vector Ri in the
argument of the wavefunction, and we have resummed the lattice vectors in
the last line with the redeﬁnition Rm = Rj − Ri.
2.1.2 Lattice with several atoms per unit cell
If we have several atoms per unit cell, such as in the case of the honeycomb
lattice, the reasoning described above must be modiﬁed. Notice ﬁrst that a
translation by any vector δj that relates a site on one sublattice to that on a
second sublattice is not a symmetry operation, i.e. [Tδj
, H] = 0, if we deﬁne
Tδj
≡ exp(iˆp · δj/¯h) in the same manner as the translation operator (2.3).
One must, therefore, treat the diﬀerent sublattices apart.
In the case of two atoms per unit cell, we may write down the trial
wavefunction as
ψk(r) = akψ
(A)
k (r) + bkψ
(B)
k (r), (2.5)
where ak and bk are complex functions of the quasi-momentum k. Both
ψ
(A)
k (r) and ψ
(B)
k (r) are Bloch functions with
ψ
(j)
k (r) =
Rl
eik·Rl
φ(j)
(r + δj − Rl), (2.6)
where j = A/B labels the atoms on the two sublattices A and B, and δj
is the vector which connects the sites of the underlying Bravais lattice with
the site of the j atom within the unit cell. Typically one chooses the sites
of one of the sublattices, e.g. the A sublattice, to coincide with the sites of
the Bravais lattice. Notice furthermore that there is some arbitrariness in
the choice of the phase in Eq. (2.6) – instead of choosing exp(ik · Rl), one
may also have chosen exp[ik · (Rl − δj), as for the arguments of the atomic
wavefunctions. The choice, however, does not aﬀect the physical properties
29.
Tight-Binding Model for Electrons on the Honeycomb Lattice 25
of the system because it simply leads to a redeﬁnition of the weights ak and
bk which aquire a diﬀerent relative phase [18].
With the help of these wavefunctions, we may now search the solutions
of the Schr¨odinger equation
Hψk = ǫkψk.
Here, we have chosen an arbitrary representation, which is not necessarily
that in real space.3
Multiplication of the Schr¨odinger equation by ψ∗
k from
the left yields the equation ψ∗
kHψk = ǫkψ∗
kψk, which may be rewritten in
matrix form with the help of Eqs. (2.5) and (2.6)
(a∗
k, b∗
k) Hk
ak
bk
= ǫk (a∗
k, b∗
k) Sk
ak
bk
. (2.7)
Here, the Hamiltonian matrix is deﬁned as
Hk ≡
ψ
(A)∗
k Hψ
(A)
k ψ
(A)∗
k Hψ
(B)
k
ψ
(B)∗
k Hψ
(A)
k ψ
(B)∗
k Hψ
(B)
k
= H†
k, (2.8)
and the overlap matrix
Sk ≡
ψ
(A)∗
k ψ
(A)
k ψ
(A)∗
k ψ
(B)
k
ψ
(B)∗
k ψ
(A)
k ψ
(B)∗
k ψ
(B)
k
= S†
k (2.9)
accounts for the non-orthogonality of the trial wavefunctions. The eigen-
values ǫk of the Schr¨odinger equation are the energy dispersions or energy
bands, and they may be obtained from the secular equation
det Hk − ǫλ
kSk = 0, (2.10)
which needs to be satisﬁed for a non-zero solution of the wavefunctions, i.e.
for ak = 0 and bk = 0. The label λ denotes the energy bands, and it is clear
that there are as many energy bands as solutions of the secular equation
(2.10), i.e. two bands for the case of two atoms per unit cell. Notice that the
generalisation to n atoms per unit cell is straight-forwards – in this case, the
wavefunction (2.5) needs to be written as
ψk =
n
j=1
a
(j)
k ψ
(j)
k ,
3
The wavefunction ψk(r) is, thus, the real space representation of the Hilbert vector
ψk.
30.
26 Electronic Band Structure of Graphene
where the superscript j denotes the diﬀerent atoms per unit cell. The secular
equation (2.10) remains valid, in terms of the Hermitian n × n matrices
Hij
k ≡ ψ
(i)∗
k Hψ
(j)
k and Sij
k ≡ ψ
(i)∗
k ψ
(j)
k , (2.11)
and it is now an equation of degree n. This means that there are n energy
bands, i.e. as many energy bands as atoms per unit cell.
In a ﬁrst step, one often neglects the overlap corrections, i.e. one assumes
a quasi-orthogonality of the wavefunctions, Sij
k = Nδij. It turns out, however,
to keep track of these overlap corrections in the case of graphene. As is
discussed in the following section, they yield a contribution which is on the
same order of magnitude as the nnn hopping corrections.
Formal solution
Before turning to the speciﬁc case of graphene and its energy bands, we solve
formally the secular equation for an arbitrary lattice with several atoms per
unit cell. The Hamiltonian matrix (2.11) may be written, with the help of
Eq. (2.6), as
Hij
k =
Rl,Rm
eik·(Rl−Rm)
d2
r φ(i)∗
(r + δi − Rk)Hφ(j)
(r + δj − Rm)
= N
kl
eik·Rl
d2
r φ(i)∗
(r) [Ha
+ ∆V ] φ(j)
(r + δij − Rl)
= N ǫ(i)
sij
k + tij
k (2.12)
where δij ≡ δj − δi,
sij
k ≡
Rl
eik·Rl
d2
r φ(i)∗
(r + δi − Rk)φ(j)
(r + δj − Rm) =
Sij
k
N
(2.13)
and we have deﬁned the hopping matrix
tij
k ≡
Rl
eik·Rl
d2
r φ(i)∗
(r + δi − Rk)∆V φ(j)
(r + δj − Rm) . (2.14)
The last line in Eq. (2.12) has been obtained from the fact that the atomic
wavefunctions φ(i)
(r) are eigenstates of the atomic Hamiltonian Ha
with the
31.
Tight-Binding Model for Electrons on the Honeycomb Lattice 27
a
a
δ
a
A
B B
B
12
3
2
1
3
3
Figure 2.1: Tight-binding model for the honeycomb lattice.
atomic energy ǫ(i)
for an orbital of type i. This atomic energy plays the role
of an onsite energy. The secular equation now reads
det tij
k − ǫλ
k − ǫ(i)
= 0. (2.15)
Notice that, if the the atoms on the diﬀerent sublattices are all of the same
electronic conﬁguration, one has ǫ(i)
= ǫ0 for all i, and one may omit this
onsite energy, which yields only a constant physically irrelevant shift of the
energy bands.
2.1.3 Solution for graphene with nearest-neighbour and
next-nearest-neighour hopping
After these formal considerations, we now study the particular case of the
tight-binding model on the honeycomb lattice, which yields, to great accu-
racy, the π energy bands of graphene. Because all atomic orbitals are pz
orbitals of carbon atoms, we may omit the onsite energy ǫ0, as discussed
in the last paragraph. We choose the Bravais lattice vectors to be those of
the A sublattice, i.e. δA = 0, and the equivalent site on the B sublattice is
obtained by the displacement δB = δAB = δ3 (see Fig. 2.1). The hopping
amplitude between nn is given by the expression
t ≡ d2
r φA∗
(r)∆V φB
(r + δ3), (2.16)
32.
28 Electronic Band Structure of Graphene
and we also take into account nnn hopping which connects nn sites on the
same sublattice
tnnn ≡ d2
r φA∗
(r)∆V φA
(r + a1) = d2
r φB∗
(r)∆V φB
(r + a1). (2.17)
Notice that one may have chosen any other vector δj or a2, respectively, in
the calculation of the hopping amplitudes. Because of the normalisation of
the atomic wavefunctions, we have d2
rφ(j)∗
(r)φ(j)
(r) = 1, and we consider
furthermore the overlap correction between orbitals on nn sites,
s ≡ d2
r φA∗
(r)φB
(r + δ3). (2.18)
We neglect overlap corrections between all other orbitals which are not nn,
as well as hopping amplitudes for larger distances than nnn.
If we now consider an arbitrary site A on the A sublattice (Fig. 2.1), we
may see that the oﬀ-diagonal terms of the hopping matrix (2.14) consist of
three terms corresponding to the nn B1, B2, and B3, all of which have the
same hopping amplitude t. However, only the site B3 is described by the
same lattice vector (shifted by δ3) as the site A and thus yields a zero phase
to the hopping matrix. The sites B1 and B2 correspond to lattice vectors
shifted by a1 and a3 ≡ a2 − a1, respectively. Therefore, they contribute
a phase factor exp(ik · a1) and exp(ik · a3), respectively. The oﬀ-diagonal
elements of the hopping matrix may therefore be written as4
tAB
k = tγ∗
k = tBA
k
∗
,
as well as those of the overlap matrix
sAB
k = sγ∗
k = sBA
k
∗
,
(sAA
k = sBB
k = 1, due to the above-mentioned normalisation of the atomic
wavefunctions), where we have deﬁned the sum of the nn phase factors
γk ≡ 1 + eik·a1
+ eik·a3
. (2.19)
4
The hopping matrix element tAB
k corresponds to a hopping from the B to the A
sublattice.
33.
Tight-Binding Model for Electrons on the Honeycomb Lattice 29
The nnn hopping amplitudes yield the diagonal elements of the hopping
matrix,
tAA
k = tBB
k = tnnn eik·a1
+ e−ik·a1
+ eik·a2
+ e−ik·a2
+ eik·a3
+ e−ik·a3
= 2tnnn
3
i=1
cos(k · ai) = tnnn |γk|2
− 3 ,
and one obtains, thus, the secular equation
det
tAA
k − ǫk (t − sǫk)γ∗
k
(t − sǫk)γk tAA
k − ǫk
= 0 (2.20)
with the two solutions (λ = ±)
ǫλ
k =
tAA
k + λt|γk|
1 + λs|γk|
. (2.21)
This expression may be expanded under the reasonable assumptions s ≪ 1
and tnnn ≪ t, which we further justify at the end of the paragraph,
ǫλ
k = tAA
k + λt|γk| − st|γk|2
= t′
nnn|γk|2
+ λt|γk|
= 2t′
nnn
3
i=1
cos(k · ai) + λt 3 + 2
3
i=1
cos(k · ai) (2.22)
where we have deﬁned the eﬀective nnn hopping amplitude
t′
nnn ≡ tnnn − st , (2.23)
and we have omitted the unimportant constant −3tnnn in the last equation.
One, therefore, notices that the overlap corrections simply yield a renor-
malisation of the nnn hopping amplitudes. The hopping amplitudes may be
determined by ﬁtting the energy dispersion (2.22) obtained within the tight-
binding approximation to those calculated numerically in more sophisticated
band-structure calculations. These yield a value of t ≃ −3 eV for the nn
hopping amplitude and t′
nnn ≃ 0.1t, which justiﬁes the above-mentioned ex-
pansion for t′
nnn/t ≪ 1. Notice that this ﬁtting procedure does not allow for
a distinction between the “true” nnn hopping amplitude tnnn and the contri-
bution from the overlap correction −st. We, therefore, omit this distinction
in the following discussion and omit the prime at the eﬀective nnn hopping
amplitude, but one should keep in mind that it is an eﬀective parameter with
a contribution from nn overlap corrections.
34.
30 Electronic Band Structure of Graphene
-2 -1 1 2 3
-2
-1
1
2
3
4(a)
(b)
π
π∗
π
π∗
Energy
K
K’
K
K’
K
K’
k
ky
x
2 31−1−2
−1
4
2
1
3
−2
Energy[inunitsoft]
wave vector
M KK Γ
Figure 2.2: Energy dispersion obtained within the tight-binding approximation, for
tnnn/t = 0.1. One distinguishes the valence (π) band from the conduction (π∗
) band. The
Fermi level is situated at the points where the π band touches the π∗
band. (a) Energy
dispersion as a function of the wave-vector components kx and ky. (b) Cut throught the
energy dispersion along characteristic lines (connecting the points K → Γ → M → K.
The energy is measured in units of t and the wave vectors in units of 1/a.
Energy dispersion of π electrons in graphene
The energy dispersion (2.22) is plotted in Fig. 2.2 for tnnn/t = 0.1. It
consists of two bands, labeled by the index λ = ±, each of which contains
the same number of states. Because each carbon atom contributes one π
electron and each electron may occupy either a spin-up or a spin-down state,
the lower band with λ = − (the π or valence band) is completely ﬁlled and
that with λ = + (the π∗
or conduction band) completely empty. The Fermi
level is, therefore, situated at the points where the π band touches the π∗
band. Notice that, if tnnn = 0, the energy dispersion (2.22) is electron-hole
symmetric, i.e. ǫλ
k = −ǫ−λ
k . This means that nnn hopping and nn overlap
corrections break the electron-hole symmetry. The points, where the π band
touches the π∗
band, are called Dirac points, for reasons that are explained
in the following chapter. They situated at the points kD
where the energy
dispersion (2.22) is zero,
ǫλ
kD = 0. (2.24)
35.
Tight-Binding Model for Electrons on the Honeycomb Lattice 31
Eq. (2.24) is satisﬁed when γkD = 0, i.e. when
ReγkD = 1 + cos(kD
· a2) + cos(kD
· a3) (2.25)
= 1 + cos
√
3a
2
(kD
x +
√
3kD
y ) + cos
√
3a
2
(−kD
x +
√
3kD
y ) = 0
and, equally,
ImγkD = sin
√
3a
2
(kD
x +
√
3kD
y ) + sin
√
3a
2
(−kD
x +
√
3kD
y ) = 0. (2.26)
The last equation may be satisﬁed by the choice kD
y = 0, and Eq. (2.25),
thus, when
1 + 2 cos
√
3a
2
kD
x = 0 ⇒ kD
x = ±
4π
3
√
3a
.
Comparison with Eq. (1.6) shows that there are, thus, two5
inequivalent
Dirac points D and D′
, which are situated at the points K and K′
, respec-
tively,
kD
= ±K = ±
4π
3
√
3a
ex. (2.27)
Although situated at the same position in the ﬁrst BZ, it is useful to make a
clear conceptual distinction between the Dirac points, which are deﬁned as
the points where the two bands π and π∗
touch each other, and the purely
crystallographic points K and K′
, which are deﬁned as the corners of the ﬁrst
BZ. There are, indeed, situations where the Dirac points move away from the
points K and K′
, e.g. when the nn hopping amplitudes are no longer the
same in the directions δ1, δ2, and δ3 [19]. In the following chapters, we will,
however, consider the natural situation for graphene where the Dirac points
are situated at the BZ corners and use the notation K and K′
for the Dirac
points.
Notice that because of the symmetry ǫ−k = ǫk, which is a consequence of
time-reversal symmetry, Dirac points occur necessarily in pairs – if kD
is a
5
We remind the reader that there are only two inequivalent points, and not six as
Fig. 2.2 (b) might suggest. As pointed out in Sec. 1.2.1, there are pairs of three points
that may be connected to one another by a reciprocal lattice vector and that are, thus,
crystallographically equivalent.
36.
32 Electronic Band Structure of Graphene
solution of ǫk = 0, so is −kD
. In graphene, there is one pair of Dirac points,
and the zero-energy states are, therefore, doubly degenerate. One speaks
of a twofold valley degeneracy, which survives when we consider low-energy
electronic excitations that are restricted to the vicinity of the Dirac points,
as is discussed in section 2.2.
Eﬀective tight-binding Hamiltonian
Before considering the low-energy excitations and the continuum limit, it is
useful to deﬁne an eﬀective tight-binding Hamiltonian,
Hk ≡ tnnn|γk|2
½ + t
0 γ∗
k
γk 0
. (2.28)
Here, ½ represents the 2 × 2 one-matrix
½ =
1 0
0 1
.
This Hamiltonian eﬀectively omits the problem of non-orthogonality of the
wavefunctions by a simple renormalisation of the nnn hopping amplitude, as
alluded to above. The eigenstates of the eﬀective Hamiltonian (2.28) are the
spinors
Ψλ
k =
aλ
k
bλ
k
, (2.29)
the components of which are the probability amplitudes of the Bloch wave-
function (2.5) on the two diﬀerent sublattices A and B. They may be deter-
mined by considering the eigenvalue equation Hk(tnnn = 0)Ψλ
k = λt|γk|Ψλ
k,
which does not take into account the nnn hopping correction. Indeed, these
eigenstates are also those of the Hamiltonian with tnnn = 0 because the nnn
term is proportional to the one-matrix ½. The solution of the eigenvalue
equation (2.29) yields
aλ
k = λ
γ∗
k
|γk|
bλ
k = λe−iϕk
bλ
k
37.
Continuum Limit 33
and, thus, the eigenstates6
Ψλ
k =
1
√
2
1
λeiϕk
, (2.30)
where we have deﬁned the angle
ϕk = arctan
Imγk
Reγk
. (2.31)
As one may have expected, the spinor represents an equal probability to
ﬁnd an electron in the state Ψλ
k on the A as on the B sublattice because both
sublattices are built from carbon atoms with the same onsite energy ǫ(i)
.7
2.2 Continuum Limit
In order to describe the low-energy excitations, i.e. electronic excitations the
characteristic energy of which is much smaller than the band width ∼ |t|,
one may concentrate on excitations at the Fermi level. This amounts to
restricting the excitations to quantum states in the vicinity of the Dirac
points, and one may expand the energy dispersion around ±K. The wave
6
The eigenstates are deﬁned up to a global (but k-dependent) phase, and one may also
choose
Ψλ
k =
1
√
2
e−iϕk
λ
,
which is also found in the litterature.
7
This is not the case for other lattices such as 2D boron nitride (BN), which also forms
a hexagonal lattice. However, in the case of BN, one sublattice consists of boron atoms
with an atomic (onsite) energy ǫA
and the other one of nitrogen atoms with an onsite
energy ǫB
= ǫA
. The diﬀerence in the onsite energy µ = ǫA
− ǫB
may be accounted for in
the eﬀective Hamiltonian (2.28) if one adds a term
µ
2
1 0
0 −1
.
This term opens a gap in the energy dispersion at the points K and K′
,
ǫλ
k = tnnn|γk|2
+ λ t2|γk|2 +
µ2
4
,
and it is energetically favourable to ﬁll preferentially the sublattice with lower onsite
energy.
38.
34 Electronic Band Structure of Graphene
vector is, thus, decomposed as k = ±K + q, where |q| ≪ |K| ∼ 1/a. The
small parameter, which governs the expansion of the energy dispersion, is,
therefore, |q|a ≪ 1.
It is evident from the form of the energy dispersion (2.22) and the eﬀective
Hamiltonian that the basic entity to be expanded is the sum of the phase
factors γk. We need to distinguish the sum at the K point from that at the
K′
point,
γ±
q ≡ γk=±K+q = 1 + e±iK·a2
eiq·a2
+ e±iK·a3
eiq·a3
≃ 1 + e±i2π/3
1 + iq · a2 −
1
2
(q · a2)2
+e∓i2π/3
1 + iq · a3 −
1
2
(q · a3)2
= γ±(0)
q + γ±(1)
q + γ±(2)
q
By deﬁnition of the Dirac points and their position at the BZ corners K and
K′
, we have γ
±(0)
q = γ±K = 0. We limit the expansion to second order in
|q|a.
First order in |q|a
The ﬁrst order term is given by
γ±(1)
q = i
√
3a
2
(qx +
√
3qy)e±i2π/3
+ (−qx +
√
3qy)e∓i2π/3
= ∓
3a
2
(qx ± iqy), (2.32)
which is obtained with the help of sin(±2π/3) = ±
√
3/2 and cos(±2π/3) =
−1/2. This yields the eﬀective low-energy Hamiltonian
Heﬀ,ξ
q = ξ¯hvF (qxσx
+ ξqyσy
), (2.33)
where we have deﬁned the Fermi velocity8
vF ≡ −
3ta
2¯h
=
3|t|a
2¯h
(2.34)
8
The minus sign in the deﬁnition is added to render the Fermi velocity positive because
the hopping parameter t ≃ −3eV happens to be negative, as mentioned in the last section.
39.
Continuum Limit 35
and the Pauli matrices
σx
=
0 1
1 0
, and
0 −i
i 0
.
Furthermore, we have introduced the valley isospin ξ = ±, where ξ = +
denotes the K point at +K and ξ = − the K′
point at −K. The low-energy
Hamiltonian (2.33) does not take into account nnn hopping corrections, which
are proportional to |γk|2
and, thus, occur only in the second-order expansion
of the energy dispersion [at order (|q|a)2
]. The energy dispersion (2.22),
therefore, reads
ǫλ
q,ξ=± = λ¯hvF |q|, (2.35)
independent of the the valley isospin ξ. We have already alluded to this
twofold valley degeneracy in Sec. 2.1.3, in the framework of the discussion
of the zero-energy states at the BZ corners. The twofold valley degeneracy,
thus, survives when considering the low-energy excitations in the vicinity of
the Dirac points. From Eq. (2.35) it is apparent that the continuum limit
|q|a ≪ 1 coincides with the limit |ǫ| ≪ |t|, as described above, because
|ǫq| = 3ta|q|/2 ≪ |t|.
It is convenient to invert the spinor components at the K′
point (for
ξ = −),
Ψk,ξ=+ =
ψA
k,+
ψB
k,+
, Ψk,ξ=− =
ψB
k,−
ψA
k,−
,
i.e. to invert the role of the two sublattices. In this case, the eﬀective low-
energy Hamiltonian may be represented as
Heﬀ,ξ
q = ξ¯hvF (qxσx
+ qyσy
) = ¯hvF τz
⊗ q · σ, (2.36)
where we have introduced the four-spinor representation
Ψk =
ψA
k,+
ψB
k,+
ψB
k,−
ψA
k,−
in the last line via the 4 × 4 matrices
τz
⊗ σ =
σ 0
0 −σ
,
40.
36 Electronic Band Structure of Graphene
and σ ≡ (σx
, σy
). In this four-spinor representation, the ﬁrst two com-
ponents represent the lattice components at the K point and the last two
components those at the K′
point. We emphasise that one must clearly dis-
tinguish both types of isospin: (a) the sublattice isospin is represented by
the Pauli matrices σj
, where “spin up” corresponds to the component on one
sublattice and “spin down” to that on the other one. A rotation within the
SU(2) sublattice isospin space yields the band indices λ = ±, and the band
index (or band isospin) is, thus, intimitely related to the sublattice isospin.
(b) The valley isospin, which is described by a second set of Pauli matrices
τj
, the z-component of which appears in the Hamiltonian (2.36), is due to
the twofold valley degeneracy and is only indirectly related to the presence
of two sublattices.
The eigenstates of the Hamiltonian (2.36) are the four-spinors
Ψξ=+
k,λ =
1
√
2
1
λeiϕq
0
0
and Ψξ=−
k,λ =
1
√
2
0
0
1
−λeiϕq
, (2.37)
where we have, now,
ϕq = arctan
qy
qx
. (2.38)
Density of states
The electronic density of states ρ(ǫ) counts the number of quantum states in
the vicinity of a ﬁxed energy ǫ. It turns out to be a very useful quantity when
discussing the electric transport in the diﬀusive regime. It may be obtained
from the total number of states below the energy ǫ,
Nλ=+
= g
k/ǫk+≤ǫ
= A
ǫ
0
dǫ′
ρ(ǫ′
), (2.39)
where we have chosen the electronic π∗
band, by derivation with respect to
the energy
ρ(ǫ) =
1
A
∂N+
∂ǫ
, (2.40)
41.
Continuum Limit 37
in terms of the total surface A.9
The factor g takes into account the de-
generacy due to internal degrees of freedom – g = 4 in the case of graphene
because of the twofold valley degeneracy and the electron spin.
The calculation of the density of states may be rather involved because
one needs to calculate a 2D integral over the wave vector as a function of
energy, by inverting the energy dispersion. In the vicinity of the Dirac points,
however, it may be calculated quite easily because of the isotropy of the
energy dispersion (2.35). One may identify
k/ǫ+
k ≤ǫ
≃
Ag
2π
q(ǫ)
0
dq q ,
where we have proﬁted from the isotropy of the energy dispersion in the
vicinity of the Dirac point, with the right hand side of Eq. (2.39), and one
obtains
ρ(ǫ) =
g
2π
q(ǫ)
∂ǫ/∂q
. (2.41)
By inverting the energy dispersion (2.35), one obtains
ρ(ǫ ≥ 0) =
gǫ
2π¯h2
v2
F
,
and for the full (positive and negative) energy range10
ρ(ǫ) =
g|ǫ|
2π¯h2
v2
F
, (2.42)
as long as |ǫ| ≪ |t|.
The density of states, therefore, vanishes linearly at the Dirac points,
at zero energy. This is a direct consequence of the linearity of the energy
dispersion in the vicinity of the Dirac points. This particular situation needs
to be contrasted to the conventional case of electrons in 2D metals, with an
energy dispersion of ǫ = ¯h2
q2
/2m∗
, in terms of the band mass m∗
, where one
obtains a constant density of states, ρ2D
(ǫ) = gm∗
/2π¯h2
.
The full density of states, in the absence of nnn hopping corrections, has
been calculated by Hobson and Nierenberger in 1953 [20]. It is schematically
9
The density of states deﬁned in this manner is indeed the density of states per unit
surface, or unit volume in 3D.
10
The negative branch of the density of states may be calculated in the same manner.
42.
38 Electronic Band Structure of Graphene
Densityofstates
Energy−t 0 t
Figure 2.3: Schematic plot of the density of states for electrons in graphene in the
absence of nnn hopping. The dashed line indicates the density of states obtained at linear
order in the continuum limit.
shown in Fig 2.3. In agreement with the result (2.42) obtained at linear order
in the continuum limit, it vanishes linearly at zero energy. The divergencies at
±t, called van-Hove singularities, are due to the saddle points of the energy
dispersion at the M points at the borders of the ﬁrst BZ (see Fig. 2.2).
This divergency may be understood qualitatively from Eq. (2.42) – roughly
speaking, the derivative of the energy dispersion occurs in the denominator
of the expression for the density of states and, thus, causes a divergency
whenever it becomes zero, such as at the extrema or saddle points of the
energy dispersion.
Second order in |q|a
Although most of the fundamental properties of graphene are captured within
the eﬀective model obtained at ﬁrst order in the expansion of the energy
dispersion, it is useful to take into account second-order terms. These cor-
rections include nnn hopping corrections and oﬀ-diagonal second-order con-
tributions from the expansion of γk. The latter yield the so-called trigonal
warping, which consist of an anisotropy of the energy dispersion around the
Dirac points.
The diagonal second-order correction, which stems from the nnn hopping,
43.
Continuum Limit 39
is readily obtained from Eq. (2.32),
Hξ
nnn = tnnn|γξ
q|2
½ ≃ tnnn|γξ(1)
q |2
½ =
9a2
4
tnnn|q|2
½. (2.43)
The oﬀ-diagonal second-order corrections are somewhat more involved
because we need to calculate the modulus of γξ
q,
|γξ
q| ≃ |γξ(1)
q |2
+ 2Reγξ(1)∗
q γξ(2)
q
1/2
≃ |γξ(1)
q | 1 +
Reγ
ξ(1)∗
q γ
ξ(2)
q
|γ
ξ(1)
q |2
.
Because of
Reγξ(1)∗
q γξ(2)
q = −ξ
9a2
16
qx(q2
x − 3q2
y) ,
one obtains at second order
|γξ
q| ≃
3a
2
|q| 1 − ξ
|q|a
4
cos(3ϕq) ,
where we have used the parametrisation qx = |q| cos ϕq and qy = |q| sin ϕq.
Finally, the energy dispersion (2.22) expanded to second order in |q|a reads
ǫλ
q,ξ =
9a2
4
tnnn|q|2
+ λ¯hvF |q| 1 − ξ
|q|a
4
cos(3ϕq) . (2.44)
As we have already mentioned in Sec. 2.1.3, it is apparent from Eq.
(2.44) that the nnn correction (which also accounts for nn overlap correc-
tions) breaks the electron-hole symmetry ǫ−λ
q,ξ = −ǫλ
q,ξ. This correction is,
however, a rather small correction, of order |q|atnnn/t, to the ﬁrst-order ef-
fective Hamiltonian (2.36). The second-order expansion of the phase factor
sum γq yields a more relevant correction – the third term in Eq. (2.44), of
order |q|a ≫ |q|atnnn/t – to the linear theory. It depends explicitely on the
valley isospin ξ and renders the energy dispersion anisotropic in q around
the K and K′
point. The tripling of the period, due to the term cos(3ϕq),
is a consequence of the symmetry of the underlying lattice and is also called
trigonal warping, as mentioned above.
The trigonal warping of the dispersion relation is visualised in Fig. 2.4,
where we have plotted the contours of constant (positive) energy in Fourier
space. The closed energy contours around the K and K′
points at low energy
are sparated by the high-energy contours around the Γ point by the dashed
44.
40 Electronic Band Structure of Graphene
-3 -2 -1 1 2 3
-3
-2
-1
1
2
3
-0.4 -0.2 0.2 0.4
-0.4
-0.2
0.2
0.4
(a) (b)
K’K’ K
q
k
k
x
y
y
x
q
1eV
1.5eV
2eV
Γ
Figure 2.4: Contours of constant (positive) energy in the wave-vector space. (a) Contours
obtained from the full dispersion relation (2.22). The dashed line corresponds to the energy
t+tnnn, which separates closed orbits around the K and K′
points (black lines, with energy
ǫ < t + tnnn) from those around the Γ point (gray line, with energy ǫ < t + tnnn). (b)
Comparison of the contours at energy ǫ = 1 eV, 1.5 eV, and 2 eV around the K′
point. The
black lines correspond to the energies calculated from the full dispersion relation (2.22)
and the gray ones to those calculated to second order within the continuum limit (2.44).
45.
Continuum Limit 41
Figure 2.5: Schematic view of an ARPES measurement (from Ref. [21]) The analyser
detects the energy Ef of the photoemitted electron as a function of the angles ϑ and ϕ,
which are related to the momentum of the electronic state.
lines in Fig. 2.4 (a) at energy |t+tnnn| the crossing points of which correspond
to the M points. As mentioned above, the dispersion relation has saddle
points at these points at the border of the ﬁrst BZ, which yield the van-
Hove singularities in the density of states (see Fig. 2.3). In Fig. 2.4 (b),
we compare constant-energy contours of the full dispersion relation to those
obtained from Eq. (2.44) calculated within a second-order expansion. The
contours are indistinguishable for an energy of ǫ = |t|/3 ≃ 1 eV, and the
continuum limit yields rather accourate results up to energies as large as 2
eV. Notice that, in today’s exfoliated graphene samples on a SiO2 substrates,
one may probe, by ﬁeld-eﬀect doping of the graphene sheet, energies which
are on the order of 100 meV. Above these energies the condenser breaks down,
and Fig. 2.4 (a) indicates that the continuum limit (2.44) yields extremely
accurate results at these energies.
2.3 Experimental Characterisation of the Elec-
tronic Band Structure
The energy dispersion relation of solids may be determined by ARPES (an-
gle resolved photoemission spectroscopy). A typical ARPES measurement
consists of the detection of the direction and energy of a photoemitted elec-
46.
42 Electronic Band Structure of Graphene
Figure 2.6: ARPES measurement of the dispersion relation of epitaxial graphene (from
Ref. [22]).
tron, i.e. an electron emitted from the solid to be studied after prior optical
excitation by a photon of well-deﬁned energy and momentum, ¯hν and ¯hk,
respectively (see Fig. 2.5). The technique, which measures the spectral func-
tion, the imaginary part of the electronic Green’s function 1/(ω−ǫkλ
+iη), is
based on energy and momentum conservation in a electron-photon scattering
process,
¯hν = Ef − Ei, k = kf − ki,
where Ei and ki represent the energy and momentum, respectively, of the
initial electronic state and Ef and kf those of the ﬁnal electronic state, i.e.
the state of the photoemitted and detected electron. The direction of the
latter, in terms of the angles ϑ and ϕ shown in Fig. 2.5, yields precisely the
momentum-dependence of the energy and thus the dispersion relation.
Fig. 2.6 shows ARPES results obtained by Bostwick et al. on epitaxial
graphene [22]. Similar results have been obtained on thin graphitic samples
[23]. The studied sample has been obtained by graphitisation of the Si-
terminated (0001) surface. Fig. 2.6 (a) shows the energy dispersion of the
π band and yields a good agreement with that calculated in Sec. 2.1.3 [see
Fig. 2.2 (b)]. In order to obtain an ARPES signal, the initial state must be
occupied, and one may see from Fig. 2.6 (a) that the Fermi level is in the π∗
band at roughly EF ≃ 0.45 eV. This is in agreement with the statement in
Sec. 1.3.2 that the graphene layer on SiC is naturally electron-doped due to
charge transfer from the SiC substrate. Fig. 2.6 (b) shows the form of the
ﬁrst BZ, which is obtained by an energy cut through the dispersion relation
at zero energy (at the Dirac points). The energy cut at the Fermi level,
EF ≃ 0.45 eV, is shown in Fig. 2.6 (b) and reveals the circular Fermi surface
around the K and K′
points. The faint satellites are due to the underlying
(hexagonal) structure of the SiC substrate.
47.
Continuum Limit 43
Finally, Fig. 2.6 (d) corresponds to a cut at −1.0 eV, i.e. in the π band at
an energy rather remote from the Dirac points. The abovementioned trigonal
warping of the Fermi surface is clearly visible at this energy.
49.
Chapter 3
The Dirac Equation for
Relativistic Fermions
As we have discussed in the last chapter, the low-energy properties of elec-
trons in graphene are described by the Hamiltonian (2.36),
Hξ
q = ξ¯hvF q · σ
which happens to be of the form of the Dirac equation describing relativistic
massless fermions. We, therefore, devote this chapter to a brief introduction
to relativistic quantum mechanics with a particular emphasis on two spatial
dimensions, which are of interest in the context of graphene. This chapter
is not meant to be a complete review of relativistic quantum mechanics of
quantum ﬁeld theory, and we refer the interested reader to more specialised
books on this fascinating ﬁeld of physics [24, 25, 26]. We have, furthermore,
tried to be as concrete as possible and to avoid formal aspects related to the
Lorentz invariance of relativistic space-time, which may be useful for high-
energy physicists but which are less relevant for condensed-matter physicists.
After retracing the historical path, which led to the elaboration of rel-
ativistic quantum mechanics and quantum ﬁeld theory in the late 20ies of
the last century, we concentrate on the particular form of the Dirac equation
in 2D (i.e. two space and one time dimensions) and its amazing physical
consequences such as the localisation problem, the resulting jittery motion
(“Zitterbewegung”), and Klein tunneling.
45
50.
46 The Dirac Equation for Relativistic Fermions
3.1 Relativistic Wave Equations
In order to obtain a relativistic wave equation, one may proceed in the same
manner as in the derivation of the Schr¨odinger equation for non-relativistic
particles from classical Hamiltonian mechanics. Remember that the classical
Hamiltonian of a particle in a potential V (r) is a function
H(p, r) =
p2
2m
+ V (r), (3.1)
deﬁned in phase space, the space spanned by the particle’s position r and
its canonical momentum p. In quantum mechanics, the position and the
momentum no longer commute, and one reinterprets Eq. (3.1) in terms of
operators acting on vectors of a Hilbert space, when one replaces
H → i¯h∂t and p → −i¯h∇ , (3.2)
where ∇ is the gradient with respect to the position r, and ∂t is the time
derivative. This procedure yields the well-known Schr¨odinger equation
i¯h∂tψ(r, t) = −
¯h
2m
∇2
+ V (r) ψ(r, t) (3.3)
of basic quantum mechanics, where the wave function ψ(r, t) is the spatial
representation of the Hilbert vector.
One may indeed apply this procedure to a free relativistic particle of mass
m the energy dispersion of which is given by
E = m2c4 + p2c2 , (3.4)
in terms of the velocity of light c. Whereas the taylor expansion for |p| ≪
mc yields the non-relativistic dispersion mc2
+ p2
/2m, apart from the mass
energy mc2
, the ultra-relativistic limit of vanishing mass yields E = c|p|.
This indicates that we need to treat, in relativistic (quantum) mechanics
the energy E and the momentum p on the same footing, in contrast to
the non-relativistic limit, where the energy is proportional to the square of
the momentum. In relativistic mechanics, one treats indeed the energy, due
to the Lorentz invariance, as the time-component of a D + 1 dimensional
momentum vector, pµ
≡ (E/c, p), or its ”covariant” vector pµ = (E/c, −p),
to account for the particular metric of the D+1-dimensional space-time. The
51.
Relativistic Wave Equations 47
k
E
−mc
mc 2
2
Figure 3.1: Dispersion relation of a relativistic particle. The dispersion consists of two
energy (positive and negative) branches, which are separated by twice the particle’s mass
energy mc2
.
energy dispersion is obtained from the Lorentz-invariant norm of this vector,
µ pµ
pµ ≡ E2
/c2
− p2
= m2
c2
, given in terms of the mass of the particle,
which is an invariant scalar with respect to the Lorentz transformations in
space-time. A slightly more detailed discussion of these aspects, concerning
the covariance of special relativity, may be found in Sec. 3.2.2.
3.1.1 Relativistic Schr¨odinger/Klein-Gordon equation
Evidently, it is more useful, in order to avoid complicated functions of diﬀer-
ential operators, to introduce the “quantum” substitution (3.2) not directly
in Eq. (3.4), but in its square. This substitution yields the equation
−¯h2
∂2
t ψ(r, t) = m2
c4
− ¯h2
c2
∇2
ψ(r, t), (3.5)
which has been derived independently by Schr¨odinger, Klein and Gordon
in 1926/27 and which is called relativistic Schr¨odinger or else Klein-Gordon
equation. The latter name is more common, and we follow this convention
here.
The Klein-Gordon equation raises, however, more puzzling questions for
the physicists of that time than it was supposed to solve. A ﬁrst consequence
of the Klein-Gordon equation is that it possesses solutions of negative energy,
52.
48 The Dirac Equation for Relativistic Fermions
as may be seen from the plane-wave ansatz
ψ(r, t) = u e−i(Et/¯h−k·r)
,
which, substituted in Eq. (3.5), yields E2
u = (m2
c4
+ ¯h2
c2
k2
)u and, thus,
the two solutions
E±
= ± m2c4 + ¯h2
c2k2, (3.6)
instead of a single positive one. Both solutions are plotted in Fig. 3.1. Notice
that negative-energy states are not problematic in a classical theory because
of the gap 2mc2
between the two energy branches – negative and positive
energy particles would simply not communicate. However, such states are a
severe problem for a quantum theory, where the ground state, alias the lowest
energy state, may not be correctly deﬁned for an energy spectrum, which has
no lower bound. A particle may, in principle, “fall” from a positive-energy
state to one of negative energy by emitting, e.g., a photon the energy of
which corresponds to the energy diﬀerence between the initial and the ﬁnal
states. We will discuss this problem in more detail in Sec. 3.3.
Another problem of the Klein-Gordon equation (3.5) is related to its
second-order time derivative. One would, in principle, need to specify not
only ψ(r, t = t0), i.e. the wave function at some reference time t0, but also
its time derivative. As a consequence, the probability density ρ(r, t), which
appears in the continuity equation
∂tρ(r, t) + ∇ · j(r, t) = 0 , (3.7)
is no longer necessarily positive, in contradiction to a physicists intuition
of a probability density. In order to illustrate this point, we consider ﬁrst
the non-relativistic Schr¨odinger equation (3.3). If we multiply Eq. (3.3) by
ψ(r, t)∗
and substract the result from the complex conjugate of Eq. (3.3)
times ψ(r, t), we obtain
i¯h [ψ(r, t)∗
∂tψ(r, t) + ψ(r, t)∂tψ(r, t)∗
]
= −
¯h2
2m
ψ(r, t)∗
∇2
ψ(r, t) − ψ(r, t)∇2
ψ(r, t)∗
or else
∂t [ψ(r, t)∗
ψ(r, t)] + ∇ · ψ(r, t)∗ ¯h
2im
∇ψ(r, t) − ψ(r, t)
¯h
2im
∇ψ(r, t)∗
= 0 .
(3.8)
53.
Relativistic Wave Equations 49
Comparison with the continuity equation (3.7) yields the probability density
ρ(r, t) = ψ(r, t)∗
ψ(r, t), (3.9)
which corresponds to the probability of ﬁnding the quantum particle at the
position r at time t, and the probability current density
j(r, t) =
¯h
2im
[ψ(r, t)∗
∇ψ(r, t) − ψ(r, t)∇ψ(r, t)∗
] . (3.10)
If we proceed in the same manner for a quantum particle described in
terms of the Klein-Gordon equation (3.5), one obtains the equation
ψ(r, t)∗
∂2
t ψ(r, t) − ψ(r, t)∂2
t ψ(r, t)∗
− c2
ψ(r, t)∗
∇2
ψ(r, t) − ψ(r, t)∇2
ψ(r, t)∗
= 0,
and the corresponding probability and probability current densities are, thus,
after multiplication of the above equation by i¯h/2mc2
,
ρ(r, t) =
i¯h
2mc2
[ψ(r, t)∗
∂tψ(r, t) − ψ(r, t)∂tψ(r, t)∗
] (3.11)
and
j(r, t) =
¯h
2im
[ψ(r, t)∗
∇ψ(r, t) − ψ(r, t)∇ψ(r, t)∗
] , (3.12)
respectively. Whereas Eq. (3.12) coincides with the probability current den-
sity (3.10) of the Schr¨odinger case, the probability density (3.11) is clearly
diﬀerent from Eq. (3.9). In contrast to our intuition and non-relativistic
quantum mechanics, this probability density may become negative, and it
is, therefore, no longer possible to interpret it as the probability of ﬁnding a
(relativistic) quantum particle at the position r at time t.
3.1.2 Dirac equation
The above-mentioned problems of the Klein-Gordon equation led Dirac, in
1928, to propose an alternative relativistic wave equation [27]. Whereas its
solutions yield positive probability densities, which are more straight-forward
to interpret physically, it did not solve the problem of negative energy states.
The latter have ﬁnally found a compelling interpretation by Dirac in terms
of anti-particles, as we will discuss later in this chapter.
54.
50 The Dirac Equation for Relativistic Fermions
In order to avoid negative probability densities, Dirac understood that
one had to search for an equation that is linear in E, i.e. of ﬁrst order in
the time derivative ∂t. For dimensional reasons, the only possible ansatz for
such an equation is
H = βmc2
+cα·p → i¯h [∂t + cα · ∇] ψ(r, t) = βmc2
ψ(r, t), (3.13)
where β and1
α = (α1, ..., αD) are dimensionless objects the mathemati-
cal properties of which are ﬁxed by the requirement that the square of the
operator equation (3.13) must satisfy the relativistic dispersion relation
E2
= m2
c4
+ c2
p2
= β2
m2
c4
+ c2
(α · p)2
+ mc3
(βα · p + α · pβ) .
In order to satisfy this equation, the introduced mathematical objects must
anti-commute,
β2
= 1, {αi, β} = 0, and {αi, αj} = 2δij, (3.14)
in terms of the anti-commutator {A, B} ≡ AB + BA. Eq. (3.14) deﬁnes
the so-called Cliﬀord algebra, and one immediately realises that the objects
β and αi must be N × N matrices, with N > 1. We summarise their main
properties.
(i) Because the Hamiltonian (3.13) is Hermitian, the matrices must be
Hermitian,
αi = α†
i and β = β†
.
(ii) Furthermore, because of α2
i = β2
= 1 [see Eq. (3.14)], the matrices
must be unitary
αi = α†
i = α−1
i , and β = β†
= β−1
,
and their eigenvalues are, therefore, ±1.
(iii) If one applies the determinant to the anti-commutator, αiαj = −αjαi,
one obtains with the help of the elementary properties of the determi-
nant,2
det(αiαj) = det(−αjαi) = (−1)N
det(αjαi) = (−1)N
det(αiαj).
In order to satisfy this equation, one needs to choose N to be even.
The lowest possible value is, therefore, N = 2.
1
One needs to introduce one αi for each space dimension.
2
We use the fact that if one multiplies an N × N matrix A by a scalar λ, one has
det(λA) = λN
det(A), and that the determinant of a product of two matrices A and B is
the product of their determinants, det(AB) = det(A) det(B).
55.
Relativistic Wave Equations 51
Inﬂuence of the space dimension on the matrix dimension N
Notice that the dimension N of the matrix must not be confunded with the
space dimension D. The latter inﬂuences, however, the possible choices for
N.
In the case of two space dimensions (D = 2), which is of interest in
graphene, we have three mutually anti-commuting objects, β, α1, and α2. It
happens that there exist, with the Pauli matrices,
σx
=
0 1
1 0
, σy
=
0 −i
i 0
, σz
=
1 0
0 −1
, (3.15)
a set of three mutually 2 × 2 matrices, which satisfy the Cliﬀord algebra
(3.14). One may identify3
β = σz
, α1 = σx
, and α2 = σy
, which yields the
2D Dirac Hamiltonian
H2D
= cσ · p + mc2
σz
, (3.16)
where σ = (σx
, σy
), as in the previous chapter. If we identify c with the Fermi
velocity vF , one immediately sees that this Hamiltonian, for m = 0, has the
same form as the eﬀective Hamiltonian (2.36) derived in the last chapter for
the description of the low-energy properties of electrons in graphene, at the
K′
point (ξ = 1). The eﬀective Hamiltonian at the K point (ξ = −1) may
be identiﬁed with a representation of the Dirac Hamiltonian in terms of the
matrices β = −σz
, α1 = −σx
, and α2 = −σy
, which are an equally valid
choice for representing the Cliﬀord algebra (3.14).
For three space dimensions (D = 3), the representation of the matrices
β and αi is slightly more involved. Whereas one may choose again the 2 × 2
Pauli matrices for zero-mass particles, i.e. when one may omit the matrix β,
H3D
m=0 = cα · p, (3.17)
with e.g. α1 = σx
, α2 = σy
, and α3 = σz
, this is no longer possible for
massive 3D particles, as may be seen from the following argument. Let
us assume that the Pauli matrices represent α1, α2, and β, respectively.
One must, therefore, ﬁnd a 2 × 2 matrix, α3, which anti-commutes with
the Pauli matrices. However, the latter also form, together with the 2 × 2
unit matrix ½, a basis of all 2 × 2 matrices. One may, thus, decompose
3
Notice that all other permutations are equally possible.
56.
52 The Dirac Equation for Relativistic Fermions
α3 = a0½ + a1σx
+ a2σy
+ a3σz
, in terms of the real numbers a0, a1, a2, and
a3. The anti-commutation requirement {α3, σi
} = 2(a0 + ai) = 0 is satisﬁed
only if we choose ai = −a0, for all values of i. However, this is at odds with
the condition α2
3 = 1 because one would have α2
3 = 2a0(2 − σx
− σy
− σz
). It
is, therefore, impossible to represent the matrices β and αi by 2×2 matrices.
Due to the condition that N must be even, the lowest possible value for
representing massive 3D particles is N = 4, and indeed one may satisfy the
Cliﬀord algebra (3.14) if one chooses, e.g., the so-called standard representa-
tion
β =
½ 0
0 −½
and αi =
0 σi
σi
0
, (3.18)
where each component is a 2 × 2 matrix, as may be veriﬁed in a straight-
forward manner. As a consequence, the Dirac Hamiltonian has also a 4 × 4
matrix structure,
H3D
m=0 =
mc2
½ cp · σ
cp · σ −mc2
½
, (3.19)
and the quantum states must be represented by 4-spinors,
Ψ =
φ
χ
(3.20)
in terms of the 2-spinors
φ =
φ1
φ2
and χ =
χ1
χ2
.
In order to obtain a better understanding of this spinor form, we may inves-
tigate the most simple case of a particle in its rest frame, i.e. with p = 0, in
which case the Hamiltonian (3.19) becomes diagonal. The 2-spinors φ and χ
are, therefore, decoupled,
mc2
φ = Eφ and − mc2
χ = Eχ.
One immediately notices that the components φ correspond to components
of positive energy (particle components) and χ to those of negative energy
(anti-particle components). One may furthermore show that the components
φ1, φ2 and χ1, χ2 of the 2-spinors φ and χ, respectively, correspond to the
diﬀerent possible spin states of the particle [24, 25].
57.
The 2D Dirac Equation 53
Continuity equation
We ﬁnally notice that the Dirac equation yields positive probability densities,
which were Dirac’s main motivation to propose an alternative to the Klein-
Gordon equation, as mentioned above. In order to obtain the continuity
equation (3.7), we proceed in the same manner as for the Schr¨odinger or
the Klein-Gordon equation, i.e. we multiply the diﬀerential equation (3.13)
from the left by the spinor ψ†
(r, t) and subtract the Hermitian conjugate of
Eq. (3.13), multiplied from the right by ψ(r, t). This yields the continuity
equation
∂t ψ†
(r, t)ψ(r, t) + c∇ · ψ†
(r, t)αψ(r, t) ,
and one thus obtains the positive probability density
ρ(r, t) = ψ†
(r, t)ψ(r, t)
and for the probability current density
j(r, t) = cψ†
(r, t)αψ(r, t).
3.2 The 2D Dirac Equation
After this short excursion to the 3D Dirac equation, we now concentrate on
the 2D equation (3.16),
H2D
= p · σ + mσz
,
which interests us in the case of graphene, where we choose a unit system
with c = ¯h = 1, for the remainder of this section. We may rewrite the
Hamiltonian as
H2D
= ǫ
cos β sin βe−iϕp
sin βeiϕp
− cos β
, (3.21)
where we have deﬁned ǫ = m2 + p2, cos β = m/ǫ, sin β = |p|/ǫ, and
ϕp = arctan(py/px), as in Eq. (2.38) for the wave vector q, which is replaced
by the momentum p. The eigenvalues of the unitary and Hermitian matrix
on the r.h.s. of Eq. (3.21) are λ = ± and correspond to the positve and
negative energy states, respectively, and we have
Eλ
= λǫ = λ m2 + p2, (3.22)
in agreement with Eq. (3.6).
58.
54 The Dirac Equation for Relativistic Fermions
3.2.1 Eigenstates of the 2D Dirac Hamiltonian
In order to obtain the eigenstates, we make the plane-wave ansatz for a
2-spinor,
Ψλ,p(r) =
1
√
2
uλ
vλ
eip·r
, (3.23)
and one obtains from its substitution in Eq. (3.21)
(cos β − λ)uλ + sin βe−iϕp
vλ = 0.
A possible choice for the 2-spinor components, which respects the normali-
sation, is
uλ = 1 + λ cos β and vλ = λ 1 − λ cos βeiϕp
,
which yields for the eigenstates
Ψλ,p(r) =
1
√
2
1 + λm√
m2+p2
λ 1 − λm√
m2+p2
eiϕp
eip·r
. (3.24)
One notices that the ultra-relativistic limit (m → 0) yields the same
states,
Ψλ,p(r) →
1
√
2
1
λeiϕp
eip·r
(3.25)
as those of low-energy electrons in graphene (2.37) if we consider one Dirac
point K or K′
. These low-energy electrons may, therefore, indeed be viewed
as massless 2D relativistic particles. In the opposite limit of large mass
(m ≫ |p|), one obtains, as in the 3D case, two decoupled equations for the
components, with
Ψλ=+,p(r) →
1
0
eip·r
,
Ψλ=−,p(r) →
0
1
eip·r
,
apart from an unimportant global phase factor in the second line. In the
case of small, but non-zero, values of the momentum, one obtains a small ad-
mixture by the “small” components vλ=+ and uλ=−. In relativistic quantum
mechanics, the components uλ=+ and vλ=− are sometimes also called “large”
components.
Be the first to comment